Download presentation

Published byMarcos Weatherington Modified over 2 years ago

1
**L2: Texture Components and Euler Angles: part 1 14th January 08**

27-750, Advanced Characterization & Microstructural Analysis A.D. (Tony) Rollett, P. Kalu

2
Lecture Objectives Show how to convert from a description of a crystal orientation based on Miller indices to matrices to Euler angles Give examples of standard named components and their associated Euler angles The overall aim is to be able to describe a texture component by a single point (in some set of coordinates such as Euler angles) instead of needing to draw the crystal embedded in a reference frame Part 1 will provide a mainly qualitative, pictorial approach to illustrate the physical meaning of Euler angles and “orientations”; part 2 will provide more mathematical detail Obj/notation AxisTransformation Matrix EulerAngles Components

3
**Miller Index Definition of a Crystal Orientation**

We use a set of three orthogonal directions as the reference frame. Mathematicians set up a set of unit vectors called e1 e2 and e3. All directions can then be described as (linear) combinations of the three basis vectors. See the Supplemental Slides for explanations of vectors and unit vectors. In many cases we use the metallurgical names Rolling Direction (RD) // e1, Transverse Direction (TD) // e2, and Normal Direction (ND) // e3. We then identify a crystal (or plane normal) parallel to 3rd axis (ND) and a crystal direction parallel to the 1st axis (RD), written as (hkl)[uvw]. The second axis is then completely specified by the other two. This situation is sometimes referred to as “biaxial texture”, to distinguish it from “uniaxial texture” in which only one crystal axis of each grain is aligned with the specimen.

4
**(Bunge) Euler Angle Definition**

The three reference axes are labeled as X, Y & Z; also commonly known as ND, RD, and TD. The three crystal axes are labeled as X’, Y’ & Z’ ; also commonly known as [100], [010] & [001] in cubic crystals. Obj/notation AxisTransformation Matrix EulerAngles Components

5
**Euler Angles, Animated e1=Xsample=RD e2=Ysample=TD e3=Zsample=ND**

Sample Axes RD TD e’1 e’2 f1 e’3= 1st position ycrystal=e2’’’ f2 xcrystal=e1’’’ zcrystal=e3’’’ = 3rd position (final) [010] [100] [001] Crystal e”2 e”3 =e”1 2nd position F

6
**Cube Texture (001)[100]: cube-on-face**

Observed in recrystallization of fcc metals The 001 orientations are parallel to the three ND, RD, and TD directions. [001] [100] [0-10] Obj/notation AxisTransformation Matrix EulerAngles Components

7
**Sharp Texture (Recrystallization)**

Look at the (001) pole figures for this type of texture: maxima correspond to {100} poles in the standard stereographic projection. Obj/notation AxisTransformation Matrix EulerAngles Components

8
**Euler angles of Cube component**

The Euler angles for this component are simple, and yet not so simple! The crystal axes align exactly with the specimen axes, therefore all three angles are exactly zero: (f1, , f2) = (0°, 0°, 0°). Matrix: Rodrigues vector: [0,0,0] Unit quaternion: [0,0,0,1] As an introduction to the effects of crystal symmetry: consider aligning [100]//TD, [010]//-RD, [001]//ND. This is evidently still the cube orientation, but the Euler angles are (f1,,f2) = (90°,0°,0°)! Obj/notation AxisTransformation Matrix EulerAngles Components

9
**{110}<001>: the Goss Component**

This type of texture is known as Goss Texture and occurs as a Recrystallization texture for FCC materials such as Brass, … In this case the (011) plane is oriented towards the ND and the [001] inside the (011) plane is along the RD. ND (110) TD [001] [100] RD Obj/notation AxisTransformation Matrix EulerAngles Components

10
**{110}<001>: cube-on-edge**

In the 011 pole figure, one of the poles is oriented parallel to the ND (center of the pole figure) but the other ones will be at 60° or 90° angles but tilted 45° from the RD! (Homework: draw the (111) pole figure) ND (110) TD [001] [100] RD {110}

11
**Euler angles of Goss component**

The Euler angles for this component are simple, and yet other variants exist, just as for the cube component. Only one rotation of 45° is needed to rotate the crystal from the reference position (i.e. the cube component) to (011)[100]; this happens to be accomplished with the 2nd Euler angle. (f1,,f2) = (0°,45°,0°). Other variants will be shown when symmetry is discussed. Matrix: Rodrigues vector: [ tan(22.5°), 0 , 0 ] Unit quaternion: [ sin(22.5°) , 0, 0, cos(22.5°)] Note that, since there is only one non-zero Euler angle, the rotation axis is obvious by inspection, i.e. the x-axis. For more general cases, the rotation axis has to be calculated. Obj/notation AxisTransformation Matrix EulerAngles Components

12
Brass component This type of texture is known as Brass Texture and occurs as a rolling texture component for materials such as Brass, Silver, and Stainless steel. Obj/notation AxisTransformation Matrix EulerAngles Components

13
Brass component, contd. The associated (110) pole figure is very similar to the Goss texture pole figure except that it is rotated about the ND. In this example, the crystal has been rotated in only one sense (anticlockwise). (100) (111) (110) Obj/notation AxisTransformation Matrix EulerAngles Components

14
**{110}<112> Brass component**

Think of rotating the Goss component around the ND. In this example, the xtal has been rotated in both senses (two variants).

15
**Brass component: Euler angles**

The brass component is convenient because we can think about performing two successive rotations: 1st about the ND, 2nd about the new position of the [100] axis. 1st rotation is 35° about the ND; 2nd rotation is 45° about the [100]. (f1,,f2) = (35°,45°,0°). Obj/notation AxisTransformation Matrix EulerAngles Components

16
**Obj/notation AxisTransformation Matrix EulerAngles Components**

17
Meaning of “Variants” The existence of variants of a given texture component is a consequence of (statistical) sample symmetry. If one permutes the Miller indices for a given component (for cubics, one can change the sign and order, but not the set of digits), then different values of the Euler angles are found for each permutation. If a pole figure is plotted of all the variants, one observes a number of physically distinct orientations, which are related to each other by symmetry operators (diads, typically) fixed in the sample frame of reference. Each physically distinct orientation is a “variant”. The number of variants listed depends on the choice of size of Euler space (typically 90x90x90°) and the alignment of the component with respect to the sample symmetry.

18
**Euler Angle Conventions**

An inconvenient fact is that the definition of Euler angles that we have given so far is not unique. Many other variants not only exist but have names and are in regular use! The differences between the conventions lie in the choice of the rotation axes (generally only the second axis) and the sense of rotation. Some of the commonly used conventions are Bunge, Roe, Kocks and Canova* (in approximate order of decreasing popularity). *You will find Canova angles inside the computer code LApp

19
**Meaning of Bunge Euler angles**

In the Bunge convention, the first two angles, f1 and F, tell you the position of the [001] crystal direction relative to the specimen axes. Think of rotating the crystal about the ND (1st angle, f1); then rotate the crystal out of the plane (about the [100] axis, F); Finally, the 3rd angle (f2) tells you how much to rotate the crystal about [001]. Obj/notation AxisTransformation Matrix EulerAngles Components

20
**Meaning of Roe Euler angles**

In the Roe convention, the first two angles, and Q, tell you the position of the [001] crystal direction relative to the specimen axes. Then think of rotating the crystal about the ND or 001 or z-axis (1st angle, ); then rotate the crystal out of the plane (about [010], or the y-axis, Q); Finally, the 3rd angle (F) tells you how much to rotate the crystal about [001]. Obj/notation AxisTransformation Matrix EulerAngles Components

21
**Meaning of Kocks Euler angles**

In the Kocks convention, which is almost the same as the Roe convention with the exception of the third angle, the first two angles, and Q, tell you the position of the [001] crystal direction relative to the specimen axes. Then think of rotating the crystal about the ND or 001 or z-axis (1st angle, ); then rotate the crystal out of the plane (about [010], or the y-axis, Q); Finally, the 3rd angle () tells you how much to counter-rotate the crystal about [001]. Here’s the difference between Roe and Kocks - the last angle is a negative or clockwise rotation about 001, instead of a positive or counter-clockwise rotation. Obj/notation AxisTransformation Matrix EulerAngles Components

22
**Kocks Euler Angles: Ship Analogy**

Analogy: position and the heading of a boat with respect to the globe. Latitude (Q) and longitude (y) describe the position of the boat; third angle describes the heading (f) of the boat relative to the line of longitude that connects the boat to the North Pole. Kocks vs. Bunge angles: to be explained later! Obj/notation AxisTransformation Matrix EulerAngles Components

23
**Euler Angle Definitions**

Kocks Bunge and Canova are inverse to one another Kocks and Roe differ by sign of third angle Bunge rotates about x’, Roe/Kocks about y’ (2nd angle) Obj/notation AxisTransformation Matrix EulerAngles Components

24
**Euler Angle Conversions**

Obj/notation AxisTransformation Matrix EulerAngles Components

25
**Complete orientations in the Pole Figure**

(f1,,f2) ~ (30°,70°,40°). Note the loss of information in a diffraction experiment if each set of poles from a single component cannot be related to one another. f2 F f1 F f2 Obj/notation AxisTransformation Matrix EulerAngles Components

26
**Complete orientations in the Inverse Pole Figure**

Think of yourself as an observer standing on the crystal axes, and measuring where the sample axes lie in relation to the crystal axes. Obj/notation AxisTransformation Matrix EulerAngles Components

27
Summary Conversion between different forms of description of texture components described. Physical picture of the meaning of Euler angles as rotations of a crystal given. Miller indices are descriptive, but matrices are useful for computation, and Euler angles are useful for mapping out textures (to be discussed).

28
Supplementary Slides The following slides provide supplementary information.

29
Miller Indices Cubic system: directions, [uvw], are equivalent to, and parallel to plane normals with the same indices, (hkl). Miller indices for a plane specify reciprocals of intercepts on each axis.

30
**Miller <-> vectors**

Miller indices [integer representation of direction cosines] can be converted to a unit vector, n, by dividing by the square root of the sum of the squares: {similar for [uvw]}. This is known as normalization.

31
**Miller Index Definition of a Texture Component**

The commonest method for specifying a texture component is the plane-direction. Specify the crystallographic plane normal that is parallel to the specimen normal (e.g. the ND) and a crystallographic direction that is parallel to the long direction (e.g. the RD). (hkl) || ND, [uvw] || RD, or (hkl)[uvw]

32
Dot Product Given two vectors, a and b, the dot product, a•b is a scalar quantity that is equal to the product of the magnitudes (lengths) of the vectors, multiplied by the cosine of the angle between them: a•b = a b cos If both vectors are unit vectors then the dot product is equal to the cosine of the angle. In index form, a•b = ai bi . Given a set of unit vectors defining an axis system, ex, ey, ez,a vector can be defined on that system by taking the dot product with each axis vector in turn, e.g.: ax = a• ex

33
**Direction Cosines Definition of direction cosines:**

The components of a unit vector are equal to the cosines of the angle between the vector and each (orthogonal, Cartesian) reference axis. We can use axis transformations to describe vectors in different reference frames (room, specimen, crystal, slip system….)

Similar presentations

OK

Wigner-Seitz Cell The Wigner–Seitz cell around a lattice point is defined as the locus of points in space that are closer to that lattice point than to.

Wigner-Seitz Cell The Wigner–Seitz cell around a lattice point is defined as the locus of points in space that are closer to that lattice point than to.

© 2018 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on limitation act 1939 Ppt on synthesis and degradation of purines and pyrimidines are what Ppt on ip address classes range Ppt on principles of peace building activities Ppt on computer malwares free Ppt on land transport Ppt on area related to circles for class 10 free download Ppt on word association testing Download ppt on civil disobedience movement in the 1960s Ppt on air pollution control act